data_2011jaa0003_cc

_audit_update_record
;
2012-06-08 # Formatted by publCIF
;
 
_audit_creation_method            SHELXL-97
_chemical_name_systematic
?
_chemical_name_common             ?
_chemical_melting_point           ?
_chemical_formula_moiety          ?
_chemical_formula_sum
 'F7 Mn3 O10 P3 Rb3'
_chemical_formula_weight          807.14
 
loop_
 _atom_type_symbol
 _atom_type_description
 _atom_type_scat_dispersion_real
 _atom_type_scat_dispersion_imag
 _atom_type_scat_source
 'O'  'O'   0.0106   0.0060
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'F'  'F'   0.0171   0.0103
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'Mn'  'Mn'   0.3368   0.7283
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'Rb'  'Rb'  -0.9393   2.9676
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'P'  'P'   0.1023   0.0942
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 
_symmetry_cell_setting            monoclinic
_symmetry_space_group_name_H-M    Cc
 
loop_
 _symmetry_equiv_pos_as_xyz
 'x, y, z'
 'x, -y, z+1/2'
 'x+1/2, y+1/2, z'
 'x+1/2, -y+1/2, z+1/2'
 
_cell_length_a                    15.1935(5)
_cell_length_b                    8.8166(2)
_cell_length_c                    12.1647(3)
_cell_angle_alpha                 90.00
_cell_angle_beta                  114.347(2)
_cell_angle_gamma                 90.00
_cell_volume                      1484.60(7)
_cell_formula_units_Z             4
_cell_measurement_temperature     120(2)
_cell_measurement_reflns_used     7760
_cell_measurement_theta_min       2.91
_cell_measurement_theta_max       27.48
 
_exptl_crystal_description        needle
_exptl_crystal_colour             brown
_exptl_crystal_size_max           0.01
_exptl_crystal_size_mid           0.01
_exptl_crystal_size_min           0.01
_exptl_crystal_density_meas       ?
_exptl_crystal_density_diffrn     3.611
_exptl_crystal_density_method     'not measured'
_exptl_crystal_F_000              1030
_exptl_absorpt_coefficient_mu     12.738
_exptl_absorpt_correction_type    multi-scan
_exptl_absorpt_correction_T_min   0.9039
_exptl_absorpt_correction_T_max   0.9039
_exptl_absorpt_process_details    ?
 
_exptl_special_details
?
 
_diffrn_ambient_temperature       120(2)
_diffrn_radiation_wavelength      0.71073
_diffrn_radiation_type            MoK\a
_diffrn_radiation_source          'Bruker-Nonius FR591 rotating anode' 
_diffrn_radiation_monochromator   '10cm confocal mirrors'
_diffrn_measurement_device_type   'Bruker-Nonius APEX II CCD camera on κ-goniostat' 
_diffrn_measurement_method         'φ & ω scans'
_diffrn_detector_area_resol_mean   '4096x4096pixels / 62x62mm'
_diffrn_standards_number          ?
_diffrn_standards_interval_count  ?
_diffrn_standards_interval_time   ?
_diffrn_standards_decay_%         ?
_diffrn_reflns_number             9424
_diffrn_reflns_av_R_equivalents   0.0533
_diffrn_reflns_av_sigmaI/netI     0.0654
_diffrn_reflns_limit_h_min        -19
_diffrn_reflns_limit_h_max        19
_diffrn_reflns_limit_k_min        -11
_diffrn_reflns_limit_k_max        11
_diffrn_reflns_limit_l_min        -15
_diffrn_reflns_limit_l_max        15
_diffrn_reflns_theta_min          2.94
_diffrn_reflns_theta_max          27.49
_reflns_number_total              3130
_reflns_number_gt                 2839
_reflns_threshold_expression      >2σ(I)
 
_computing_data_collection        ?
_computing_cell_refinement        ?
_computing_data_reduction         ?
_computing_structure_solution     ?
_computing_structure_refinement   'SHELXL-97 (Sheldrick, 2008)'
_computing_molecular_graphics     ?
_computing_publication_material   ?
 
_refine_special_details
;
 Refinement of F² against ALL reflections.  The weighted R-factor wR and
 goodness of fit S are based on F², conventional R-factors R are based
 on F, with F set to zero for negative F². The threshold expression of
 F² > 2σ(F²) is used only for calculating R-factors(gt) etc. and is
 not relevant to the choice of reflections for refinement.  R-factors based
 on F² are statistically about twice as large as those based on F, and R-
 factors based on ALL data will be even larger.
;
 
_refine_ls_structure_factor_coef  Fsqd
_refine_ls_matrix_type            full
_refine_ls_weighting_scheme       calc
_refine_ls_weighting_details
 'calc w=1/[σ²(Fo²)+(0.0819P)²+96.0600P] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary      direct
_atom_sites_solution_secondary    difmap
_refine_ls_extinction_method      none
_refine_ls_extinction_coef        ?
_refine_ls_abs_structure_details
 'Flack H D (1983), Acta Cryst. A39, 876-881'
_refine_ls_abs_structure_Flack    0.78(2)
_refine_ls_number_reflns          3130
_refine_ls_number_parameters      235
_refine_ls_number_restraints      2
_refine_ls_R_factor_all           0.0721
_refine_ls_R_factor_gt            0.0649
_refine_ls_wR_factor_ref          0.1637
_refine_ls_wR_factor_gt           0.1576
_refine_ls_goodness_of_fit_ref    1.033
_refine_ls_restrained_S_all       1.032
_refine_ls_shift/su_max           0.000
_refine_ls_shift/su_mean          0.000
 
loop_
 _atom_site_label
 _atom_site_type_symbol
 _atom_site_fract_x
 _atom_site_fract_y
 _atom_site_fract_z
 _atom_site_U_iso_or_equiv
 _atom_site_adp_type
 _atom_site_occupancy
 _atom_site_symmetry_multiplicity
 _atom_site_calc_flag
 _atom_site_refinement_flags
 _atom_site_disorder_assembly
 _atom_site_disorder_group
P1 P 0.3619(3) 0.9204(4) 0.3964(3) 0.0082(7) Uani 1 1 d . . .
P2 P -0.0330(3) 0.9148(5) 0.2113(4) 0.0163(8) Uani 1 1 d . . .
P3 P 0.1329(3) 0.4188(5) 0.2077(3) 0.0153(8) Uani 1 1 d . . .
F1 F 0.0850(6) 1.0797(10) 0.0410(7) 0.0140(17) Uani 1 1 d . . .
O1 O 0.3478(8) 0.7545(12) 0.3543(9) 0.012(2) Uani 1 1 d . . .
O2 O 0.2651(7) 1.0049(11) 0.3571(8) 0.0075(18) Uani 1 1 d . . .
F2 F -0.2152(8) 0.6014(11) 0.1450(8) 0.023(2) Uani 1 1 d . . .
O3 O 0.4299(7) 1.0010(12) 0.3500(9) 0.014(2) Uani 1 1 d . . .
F3 F 0.0872(8) 0.4183(12) 0.0672(8) 0.023(2) Uani 1 1 d . . .
F4 F 0.3714(7) 0.8173(12) 0.1472(9) 0.024(2) Uani 1 1 d . . .
F5 F 0.2421(7) 0.5992(11) 0.0417(8) 0.0169(18) Uani 1 1 d . . .
O4 O 0.4129(8) 0.9202(13) 0.5340(9) 0.016(2) Uani 1 1 d . . .
F6 F -0.0810(8) 0.9178(12) 0.0699(9) 0.023(2) Uani 1 1 d . . .
F7 F 0.1873(7) 0.8352(12) 0.1514(8) 0.022(2) Uani 1 1 d . . .
O5 O 0.1703(9) 0.2606(13) 0.2483(10) 0.020(2) Uani 1 1 d . . .
O6 O 0.0685(8) 0.9766(16) 0.2512(9) 0.022(3) Uani 1 1 d . . .
O7 O -0.0936(9) 1.0169(13) 0.2512(10) 0.021(2) Uani 1 1 d . . .
O8 O 0.2143(9) 0.5313(13) 0.2492(11) 0.022(2) Uani 1 1 d . . .
O9 O 0.0565(9) 0.4650(15) 0.2481(10) 0.025(3) Uani 1 1 d . . .
O10 O -0.0319(10) 0.7544(14) 0.2504(11) 0.027(3) Uani 1 1 d . . .
Mn1 Mn 0.17144(15) 1.0454(3) 0.19597(19) 0.0093(4) Uani 1 1 d . . .
Rb1 Rb 0.17593(10) 0.71667(18) 0.42577(12) 0.0151(3) Uani 1 1 d . . .
Rb2 Rb 0.37613(12) 0.31310(15) 0.42762(14) 0.0150(3) Uani 1 1 d . . .
Rb3 Rb 0.06736(10) 0.21617(19) 0.41622(12) 0.0168(3) Uani 1 1 d . . .
Mn2 Mn -0.08094(15) 0.5402(2) 0.19018(18) 0.0088(4) Uani 1 1 d . . .
Mn3 Mn 0.29393(18) 0.6685(2) 0.1946(2) 0.0096(4) Uani 1 1 d . . .
 
 
_geom_special_details
;
 All s.u.'s (except the s.u. in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell s.u.'s are taken
 into account individually in the estimation of s.u.'s in distances, angles
 and torsion angles; correlations between s.u.'s in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell s.u.'s is used for estimating s.u.'s involving l.s. planes.
;
 
loop_
 _geom_bond_atom_site_label_1
 _geom_bond_atom_site_label_2
 _geom_bond_distance
 _geom_bond_site_symmetry_2
 _geom_bond_publ_flag
P1 O4 1.527(11) . ?
P1 O1 1.536(11) . ?
P1 O2 1.537(10) . ?
P1 O3 1.540(10) . ?
P1 Rb2 3.480(4) 1_565 ?
P1 Rb1 3.488(4) . ?
P1 Rb3 3.526(4) 3 ?
P2 O10 1.491(13) . ?
P2 O7 1.505(11) . ?
P2 O6 1.514(12) . ?
P2 F6 1.567(10) . ?
P2 Rb3 3.531(4) 1_565 ?
P2 Rb2 3.554(4) 3_455 ?
P2 Rb1 3.621(5) . ?
P2 Rb2 3.954(4) 4_464 ?
P3 O9 1.491(12) . ?
P3 O8 1.502(12) . ?
P3 O5 1.510(12) . ?
P3 F3 1.557(10) . ?
P3 Rb3 3.564(4) . ?
P3 Rb1 3.596(4) . ?
P3 Rb2 3.678(4) . ?
P3 Rb1 3.933(4) 2_564 ?
F1 Mn1 1.825(9) . ?
F1 Rb1 2.948(9) 2_574 ?
F1 Rb3 2.974(9) 2_564 ?
F1 Rb2 3.043(9) 4_464 ?
O1 Mn3 1.926(10) . ?
O1 Rb1 3.091(10) . ?
O1 Rb3 3.120(11) 3 ?
O2 Mn1 1.922(9) . ?
O2 Rb2 3.126(9) 1_565 ?
O2 Rb1 3.151(9) . ?
F2 Mn2 1.957(11) . ?
F2 Mn1 2.116(11) 3_445 ?
F2 Rb1 2.964(9) 4_464 ?
O3 Mn2 1.914(10) 3 ?
O3 Rb2 3.125(11) 1_565 ?
O3 Rb3 3.152(11) 3 ?
F3 Rb1 2.847(10) 2_564 ?
F3 Rb2 3.584(11) 4_454 ?
F4 Mn3 2.000(10) . ?
F4 Mn2 2.084(11) 3 ?
F4 Rb2 2.937(10) 2_564 ?
F4 Rb3 3.512(10) 3 ?
F5 Mn3 1.801(9) . ?
F5 Rb3 2.947(9) 2_564 ?
F5 Rb2 3.000(9) 2_564 ?
F5 Rb1 3.096(9) 2_564 ?
O4 Mn2 1.896(10) 4_565 ?
F6 Rb2 2.850(10) 4_464 ?
F6 Rb1 3.574(10) 4_464 ?
F7 Mn1 1.973(11) . ?
F7 Mn3 2.088(11) . ?
F7 Rb3 2.722(9) 2_564 ?
F7 Rb1 3.569(9) . ?
O5 Mn1 2.004(11) 1_545 ?
O5 Rb2 3.021(12) . ?
O5 Rb3 3.068(12) . ?
O6 Mn1 2.033(11) . ?
O6 Rb3 2.919(13) 1_565 ?
O6 Rb1 3.094(12) . ?
O7 Mn3 2.052(12) 3_455 ?
O7 Rb2 2.976(12) 3_455 ?
O7 Rb3 3.008(13) 1_565 ?
O8 Mn3 2.007(12) . ?
O8 Rb1 2.943(12) . ?
O8 Rb2 3.171(13) . ?
O9 Mn2 2.021(13) . ?
O9 Rb3 2.957(12) . ?
O9 Rb1 3.107(13) . ?
O10 Mn2 2.052(13) . ?
O10 Rb1 3.013(14) . ?
O10 Rb2 3.058(13) 3_455 ?
Mn1 O5 2.004(11) 1_565 ?
Mn1 F2 2.116(11) 3 ?
Mn1 Rb3 3.868(3) 2_564 ?
Mn1 Rb1 3.924(3) 2_574 ?
Mn1 Rb3 3.929(3) 1_565 ?
Mn1 Rb2 3.995(3) 1_565 ?
Mn1 Rb1 4.008(3) . ?
Rb1 F3 2.847(10) 2_565 ?
Rb1 F1 2.948(9) 2_575 ?
Rb1 F2 2.964(9) 4_565 ?
Rb1 F5 3.096(9) 2_565 ?
Rb2 F6 2.850(10) 4_565 ?
Rb2 F4 2.937(10) 2_565 ?
Rb2 O7 2.976(12) 3_545 ?
Rb2 F5 3.000(9) 2_565 ?
Rb2 F1 3.043(9) 4_565 ?
Rb2 O10 3.058(13) 3_545 ?
Rb2 O3 3.125(11) 1_545 ?
Rb2 O2 3.126(10) 1_545 ?
Rb2 P1 3.480(4) 1_545 ?
Rb2 P2 3.554(4) 3_545 ?
Rb3 F7 2.722(9) 2_565 ?
Rb3 O6 2.919(13) 1_545 ?
Rb3 F5 2.947(9) 2_565 ?
Rb3 F1 2.974(9) 2_565 ?
Rb3 O7 3.008(13) 1_545 ?
Rb3 O1 3.120(11) 3_445 ?
Rb3 O3 3.152(11) 3_445 ?
Rb3 F4 3.512(10) 3_445 ?
Rb3 P1 3.526(4) 3_445 ?
Rb3 P2 3.531(4) 1_545 ?
Mn2 O4 1.896(10) 4_464 ?
Mn2 O3 1.914(10) 3_445 ?
Mn2 F4 2.084(11) 3_445 ?
Mn2 Rb2 4.014(3) 3_455 ?
Mn2 Rb2 4.314(3) 4_454 ?
Mn2 Rb1 4.335(3) 4_464 ?
Mn3 O7 2.052(12) 3_545 ?
Mn3 Rb3 3.839(3) 2_564 ?
Mn3 Rb3 3.933(3) 3 ?
Mn3 Rb2 3.934(3) 2_564 ?
 
loop_
 _geom_angle_atom_site_label_1
 _geom_angle_atom_site_label_2
 _geom_angle_atom_site_label_3
 _geom_angle
 _geom_angle_site_symmetry_1
 _geom_angle_site_symmetry_3
 _geom_angle_publ_flag
O4 P1 O1 107.6(6) . . ?
O4 P1 O2 109.3(6) . . ?
O1 P1 O2 112.0(6) . . ?
O4 P1 O3 106.7(6) . . ?
O1 P1 O3 109.8(6) . . ?
O2 P1 O3 111.2(6) . . ?
O4 P1 Rb2 84.3(5) . 1_565 ?
O1 P1 Rb2 168.0(4) . 1_565 ?
O2 P1 Rb2 63.9(4) . 1_565 ?
O3 P1 Rb2 63.9(4) . 1_565 ?
O4 P1 Rb1 87.4(4) . . ?
O1 P1 Rb1 62.4(4) . . ?
O2 P1 Rb1 64.6(4) . . ?
O3 P1 Rb1 165.7(4) . . ?
Rb2 P1 Rb1 121.20(11) 1_565 . ?
O4 P1 Rb3 83.6(4) . 3 ?
O1 P1 Rb3 62.2(4) . 3 ?
O2 P1 Rb3 167.1(4) . 3 ?
O3 P1 Rb3 63.4(4) . 3 ?
Rb2 P1 Rb3 119.15(11) 1_565 3 ?
Rb1 P1 Rb3 117.50(10) . 3 ?
O10 P2 O7 113.1(7) . . ?
O10 P2 O6 111.3(8) . . ?
O7 P2 O6 111.1(7) . . ?
O10 P2 F6 107.8(7) . . ?
O7 P2 F6 106.0(6) . . ?
O6 P2 F6 107.3(6) . . ?
O10 P2 Rb3 122.9(5) . 1_565 ?
O7 P2 Rb3 57.7(5) . 1_565 ?
O6 P2 Rb3 54.3(5) . 1_565 ?
F6 P2 Rb3 129.3(4) . 1_565 ?
O10 P2 Rb2 58.7(5) . 3_455 ?
O7 P2 Rb2 55.6(5) . 3_455 ?
O6 P2 Rb2 120.5(4) . 3_455 ?
F6 P2 Rb2 132.0(4) . 3_455 ?
Rb3 P2 Rb2 81.58(9) 1_565 3_455 ?
O10 P2 Rb1 54.6(6) . . ?
O7 P2 Rb1 121.8(5) . . ?
O6 P2 Rb1 57.9(5) . . ?
F6 P2 Rb1 132.2(4) . . ?
Rb3 P2 Rb1 81.90(10) 1_565 . ?
Rb2 P2 Rb1 80.64(9) 3_455 . ?
O10 P2 Rb2 144.0(5) . 4_464 ?
O7 P2 Rb2 83.1(5) . 4_464 ?
O6 P2 Rb2 90.3(5) . 4_464 ?
F6 P2 Rb2 36.4(4) . 4_464 ?
Rb3 P2 Rb2 93.07(10) 1_565 4_464 ?
Rb2 P2 Rb2 134.17(13) 3_455 4_464 ?
Rb1 P2 Rb2 143.95(12) . 4_464 ?
O9 P3 O8 110.7(7) . . ?
O9 P3 O5 112.6(7) . . ?
O8 P3 O5 110.7(7) . . ?
O9 P3 F3 107.9(7) . . ?
O8 P3 F3 107.6(7) . . ?
O5 P3 F3 107.1(6) . . ?
O9 P3 Rb3 54.5(5) . . ?
O8 P3 Rb3 121.7(5) . . ?
O5 P3 Rb3 58.8(5) . . ?
F3 P3 Rb3 130.6(5) . . ?
O9 P3 Rb1 59.1(5) . . ?
O8 P3 Rb1 52.8(5) . . ?
O5 P3 Rb1 120.2(5) . . ?
F3 P3 Rb1 132.5(4) . . ?
Rb3 P3 Rb1 81.97(9) . . ?
O9 P3 Rb2 121.0(5) . . ?
O8 P3 Rb2 58.8(5) . . ?
O5 P3 Rb2 53.0(5) . . ?
F3 P3 Rb2 131.1(4) . . ?
Rb3 P3 Rb2 81.20(9) . . ?
Rb1 P3 Rb2 79.97(9) . . ?
O9 P3 Rb1 143.3(5) . 2_564 ?
O8 P3 Rb1 94.8(5) . 2_564 ?
O5 P3 Rb1 80.2(5) . 2_564 ?
F3 P3 Rb1 37.0(4) . 2_564 ?
Rb3 P3 Rb1 131.63(13) . 2_564 ?
Rb1 P3 Rb1 145.09(13) . 2_564 ?
Rb2 P3 Rb1 94.53(10) . 2_564 ?
Mn1 F1 Rb1 108.3(4) . 2_574 ?
Mn1 F1 Rb3 104.9(4) . 2_564 ?
Rb1 F1 Rb3 104.7(3) 2_574 2_564 ?
Mn1 F1 Rb2 133.7(4) . 4_464 ?
Rb1 F1 Rb2 101.6(3) 2_574 4_464 ?
Rb3 F1 Rb2 100.6(2) 2_564 4_464 ?
P1 O1 Mn3 130.9(6) . . ?
P1 O1 Rb1 91.5(4) . . ?
Mn3 O1 Rb1 100.6(4) . . ?
P1 O1 Rb3 92.0(5) . 3 ?
Mn3 O1 Rb3 99.7(4) . 3 ?
Rb1 O1 Rb3 149.7(4) . 3 ?
P1 O2 Mn1 128.2(6) . . ?
P1 O2 Rb2 89.8(4) . 1_565 ?
Mn1 O2 Rb2 102.0(4) . 1_565 ?
P1 O2 Rb1 89.3(4) . . ?
Mn1 O2 Rb1 101.6(4) . . ?
Rb2 O2 Rb1 150.5(3) 1_565 . ?
Mn2 F2 Mn1 137.2(5) . 3_445 ?
Mn2 F2 Rb1 122.2(4) . 4_464 ?
Mn1 F2 Rb1 99.8(4) 3_445 4_464 ?
P1 O3 Mn2 131.7(6) . 3 ?
P1 O3 Rb2 89.8(5) . 1_565 ?
Mn2 O3 Rb2 103.0(4) 3 1_565 ?
P1 O3 Rb3 90.7(5) . 3 ?
Mn2 O3 Rb3 100.0(4) 3 3 ?
Rb2 O3 Rb3 148.5(4) 1_565 3 ?
P3 F3 Rb1 123.8(5) . 2_564 ?
P3 F3 Rb2 115.4(5) . 4_454 ?
Rb1 F3 Rb2 91.7(3) 2_564 4_454 ?
Mn3 F4 Mn2 137.0(5) . 3 ?
Mn3 F4 Rb2 104.1(4) . 2_564 ?
Mn2 F4 Rb2 117.4(4) 3 2_564 ?
Mn3 F4 Rb3 86.5(3) . 3 ?
Mn2 F4 Rb3 86.1(3) 3 3 ?
Rb2 F4 Rb3 114.8(3) 2_564 3 ?
Mn3 F5 Rb3 105.3(4) . 2_564 ?
Mn3 F5 Rb2 107.4(4) . 2_564 ?
Rb3 F5 Rb2 104.9(3) 2_564 2_564 ?
Mn3 F5 Rb1 134.2(4) . 2_564 ?
Rb3 F5 Rb1 101.9(3) 2_564 2_564 ?
Rb2 F5 Rb1 100.1(3) 2_564 2_564 ?
P1 O4 Mn2 153.0(7) . 4_565 ?
P2 F6 Rb2 124.5(5) . 4_464 ?
P2 F6 Rb1 116.9(5) . 4_464 ?
Rb2 F6 Rb1 92.7(3) 4_464 4_464 ?
Mn1 F7 Mn3 139.6(5) . . ?
Mn1 F7 Rb3 109.9(4) . 2_564 ?
Mn3 F7 Rb3 105.2(4) . 2_564 ?
Mn1 F7 Rb1 87.7(3) . . ?
Mn3 F7 Rb1 83.7(3) . . ?
Rb3 F7 Rb1 131.6(3) 2_564 . ?
P3 O5 Mn1 145.3(7) . 1_545 ?
P3 O5 Rb2 103.5(6) . . ?
Mn1 O5 Rb2 103.5(4) 1_545 . ?
P3 O5 Rb3 96.2(6) . . ?
Mn1 O5 Rb3 99.4(4) 1_545 . ?
Rb2 O5 Rb3 101.5(3) . . ?
P2 O6 Mn1 145.3(7) . . ?
P2 O6 Rb3 100.8(6) . 1_565 ?
Mn1 O6 Rb3 103.6(5) . 1_565 ?
P2 O6 Rb1 97.7(6) . . ?
Mn1 O6 Rb1 100.8(4) . . ?
Rb3 O6 Rb1 102.4(3) 1_565 . ?
P2 O7 Mn3 144.8(7) . 3_455 ?
P2 O7 Rb2 99.7(6) . 3_455 ?
Mn3 O7 Rb2 106.3(5) 3_455 3_455 ?
P2 O7 Rb3 97.3(6) . 1_565 ?
Mn3 O7 Rb3 100.3(4) 3_455 1_565 ?
Rb2 O7 Rb3 101.3(3) 3_455 1_565 ?
P3 O8 Mn3 144.3(8) . . ?
P3 O8 Rb1 103.2(6) . . ?
Mn3 O8 Rb1 103.6(4) . . ?
P3 O8 Rb2 97.4(6) . . ?
Mn3 O8 Rb2 100.9(5) . . ?
Rb1 O8 Rb2 99.7(4) . . ?
P3 O9 Mn2 143.8(7) . . ?
P3 O9 Rb3 101.3(6) . . ?
Mn2 O9 Rb3 103.8(5) . . ?
P3 O9 Rb1 96.5(6) . . ?
Mn2 O9 Rb1 103.4(5) . . ?
Rb3 O9 Rb1 101.5(3) . . ?
P2 O10 Mn2 143.6(8) . . ?
P2 O10 Rb1 101.6(7) . . ?
Mn2 O10 Rb1 105.8(5) . . ?
P2 O10 Rb2 96.7(6) . 3_455 ?
Mn2 O10 Rb2 101.7(5) . 3_455 ?
Rb1 O10 Rb2 99.8(4) . 3_455 ?
F1 Mn1 O2 177.9(4) . . ?
F1 Mn1 F7 89.4(4) . . ?
O2 Mn1 F7 89.0(4) . . ?
F1 Mn1 O5 94.3(4) . 1_565 ?
O2 Mn1 O5 87.2(4) . 1_565 ?
F7 Mn1 O5 174.0(5) . 1_565 ?
F1 Mn1 O6 93.8(4) . . ?
O2 Mn1 O6 87.4(4) . . ?
F7 Mn1 O6 90.5(5) . . ?
O5 Mn1 O6 94.0(5) 1_565 . ?
F1 Mn1 F2 89.1(4) . 3 ?
O2 Mn1 F2 89.5(4) . 3 ?
F7 Mn1 F2 86.1(4) . 3 ?
O5 Mn1 F2 89.2(5) 1_565 3 ?
O6 Mn1 F2 175.5(5) . 3 ?
F1 Mn1 Rb3 48.0(3) . 2_564 ?
O2 Mn1 Rb3 130.4(3) . 2_564 ?
F7 Mn1 Rb3 41.4(3) . 2_564 ?
O5 Mn1 Rb3 142.2(3) 1_565 2_564 ?
O6 Mn1 Rb3 91.2(4) . 2_564 ?
F2 Mn1 Rb3 88.2(3) 3 2_564 ?
F1 Mn1 Rb1 45.5(3) . 2_574 ?
O2 Mn1 Rb1 133.8(3) . 2_574 ?
F7 Mn1 Rb1 103.0(3) . 2_574 ?
O5 Mn1 Rb1 76.4(3) 1_565 2_574 ?
O6 Mn1 Rb1 135.9(3) . 2_574 ?
F2 Mn1 Rb1 48.1(3) 3 2_574 ?
Rb3 Mn1 Rb1 73.96(5) 2_564 2_574 ?
F1 Mn1 Rb3 108.7(3) . 1_565 ?
O2 Mn1 Rb3 73.3(3) . 1_565 ?
F7 Mn1 Rb3 132.6(3) . 1_565 ?
O5 Mn1 Rb3 50.4(3) 1_565 1_565 ?
O6 Mn1 Rb3 46.2(4) . 1_565 ?
F2 Mn1 Rb3 135.7(3) 3 1_565 ?
Rb3 Mn1 Rb3 134.01(7) 2_564 1_565 ?
Rb1 Mn1 Rb3 121.14(7) 2_574 1_565 ?
F1 Mn1 Rb2 130.6(3) . 1_565 ?
O2 Mn1 Rb2 50.0(3) . 1_565 ?
F7 Mn1 Rb2 126.9(3) . 1_565 ?
O5 Mn1 Rb2 47.3(3) 1_565 1_565 ?
O6 Mn1 Rb2 115.1(3) . 1_565 ?
F2 Mn1 Rb2 65.0(3) 3 1_565 ?
Rb3 Mn1 Rb2 152.86(7) 2_564 1_565 ?
Rb1 Mn1 Rb2 89.87(5) 2_574 1_565 ?
Rb3 Mn1 Rb2 73.00(5) 1_565 1_565 ?
F1 Mn1 Rb1 129.7(3) . . ?
O2 Mn1 Rb1 50.4(3) . . ?
F7 Mn1 Rb1 62.9(3) . . ?
O5 Mn1 Rb1 117.6(3) 1_565 . ?
O6 Mn1 Rb1 49.3(3) . . ?
F2 Mn1 Rb1 126.3(3) 3 . ?
Rb3 Mn1 Rb1 93.77(6) 2_564 . ?
Rb1 Mn1 Rb1 165.89(7) 2_574 . ?
Rb3 Mn1 Rb1 72.39(5) 1_565 . ?
Rb2 Mn1 Rb1 98.67(6) 1_565 . ?
F3 Rb1 O8 119.7(3) 2_565 . ?
F3 Rb1 F1 62.4(3) 2_565 2_575 ?
O8 Rb1 F1 163.3(3) . 2_575 ?
F3 Rb1 F2 84.8(3) 2_565 4_565 ?
O8 Rb1 F2 138.8(3) . 4_565 ?
F1 Rb1 F2 55.9(3) 2_575 4_565 ?
F3 Rb1 O10 81.7(3) 2_565 . ?
O8 Rb1 O10 90.6(3) . . ?
F1 Rb1 O10 73.1(3) 2_575 . ?
F2 Rb1 O10 127.6(3) 4_565 . ?
F3 Rb1 O1 151.7(3) 2_565 . ?
O8 Rb1 O1 53.8(3) . . ?
F1 Rb1 O1 133.1(3) 2_575 . ?
F2 Rb1 O1 88.4(3) 4_565 . ?
O10 Rb1 O1 123.3(3) . . ?
F3 Rb1 O6 118.5(3) 2_565 . ?
O8 Rb1 O6 96.8(3) . . ?
F1 Rb1 O6 69.9(3) 2_575 . ?
F2 Rb1 O6 99.1(3) 4_565 . ?
O10 Rb1 O6 47.9(3) . . ?
O1 Rb1 O6 89.7(3) . . ?
F3 Rb1 F5 59.6(3) 2_565 2_565 ?
O8 Rb1 F5 73.0(3) . 2_565 ?
F1 Rb1 F5 117.3(2) 2_575 2_565 ?
F2 Rb1 F5 96.9(2) 4_565 2_565 ?
O10 Rb1 F5 118.1(3) . 2_565 ?
O1 Rb1 F5 94.1(3) . 2_565 ?
O6 Rb1 F5 163.6(3) . 2_565 ?
F3 Rb1 O9 80.5(3) 2_565 . ?
O8 Rb1 O9 47.9(3) . . ?
F1 Rb1 O9 120.8(3) 2_575 . ?
F2 Rb1 O9 164.1(3) 4_565 . ?
O10 Rb1 O9 56.3(3) . . ?
O1 Rb1 O9 101.5(3) . . ?
O6 Rb1 O9 93.4(3) . . ?
F5 Rb1 O9 70.2(3) 2_565 . ?
F3 Rb1 O2 149.3(3) 2_565 . ?
O8 Rb1 O2 91.0(3) . . ?
F1 Rb1 O2 88.4(2) 2_575 . ?
F2 Rb1 O2 70.2(3) 4_565 . ?
O10 Rb1 O2 99.4(3) . . ?
O1 Rb1 O2 48.2(3) . . ?
O6 Rb1 O2 51.9(3) . . ?
F5 Rb1 O2 138.7(2) 2_565 . ?
O9 Rb1 O2 125.7(3) . . ?
F3 Rb1 P1 151.9(2) 2_565 . ?
O8 Rb1 P1 78.4(2) . . ?
F1 Rb1 P1 107.02(19) 2_575 . ?
F2 Rb1 P1 68.8(2) 4_565 . ?
O10 Rb1 P1 121.8(2) . . ?
O1 Rb1 P1 26.1(2) . . ?
O6 Rb1 P1 76.6(2) . . ?
F5 Rb1 P1 112.66(18) 2_565 . ?
O9 Rb1 P1 124.2(2) . . ?
O2 Rb1 P1 26.15(18) . . ?
F3 Rb1 F7 154.8(3) 2_565 . ?
O8 Rb1 F7 51.6(3) . . ?
F1 Rb1 F7 118.6(2) 2_575 . ?
F2 Rb1 F7 117.3(2) 4_565 . ?
O10 Rb1 F7 75.3(3) . . ?
O1 Rb1 F7 48.2(3) . . ?
O6 Rb1 F7 49.9(3) . . ?
F5 Rb1 F7 123.9(2) 2_565 . ?
O9 Rb1 F7 78.3(3) . . ?
O2 Rb1 F7 47.5(2) . . ?
P1 Rb1 F7 53.14(16) . . ?
F6 Rb2 F4 81.9(3) 4_565 2_565 ?
F6 Rb2 O7 82.6(3) 4_565 3_545 ?
F4 Rb2 O7 164.0(3) 2_565 3_545 ?
F6 Rb2 F5 62.2(3) 4_565 2_565 ?
F4 Rb2 F5 53.4(3) 2_565 2_565 ?
O7 Rb2 F5 120.9(3) 3_545 2_565 ?
F6 Rb2 O5 118.4(3) 4_565 . ?
F4 Rb2 O5 101.0(3) 2_565 . ?
O7 Rb2 O5 89.6(3) 3_545 . ?
F5 Rb2 O5 71.1(3) 2_565 . ?
F6 Rb2 F1 62.1(3) 4_565 4_565 ?
F4 Rb2 F1 97.0(3) 2_565 4_565 ?
O7 Rb2 F1 72.4(3) 3_545 4_565 ?
F5 Rb2 F1 119.4(2) 2_565 4_565 ?
O5 Rb2 F1 161.9(3) . 4_565 ?
F6 Rb2 O10 120.8(3) 4_565 3_545 ?
F4 Rb2 O10 139.9(3) 2_565 3_545 ?
O7 Rb2 O10 48.9(3) 3_545 3_545 ?
F5 Rb2 O10 164.6(3) 2_565 3_545 ?
O5 Rb2 O10 95.9(3) . 3_545 ?
F1 Rb2 O10 71.2(3) 4_565 3_545 ?
F6 Rb2 O3 153.4(3) 4_565 1_545 ?
F4 Rb2 O3 92.1(3) 2_565 1_545 ?
O7 Rb2 O3 100.2(3) 3_545 1_545 ?
F5 Rb2 O3 132.7(3) 2_565 1_545 ?
O5 Rb2 O3 88.2(3) . 1_545 ?
F1 Rb2 O3 93.2(3) 4_565 1_545 ?
O10 Rb2 O3 52.1(3) 3_545 1_545 ?
F6 Rb2 O2 148.5(3) 4_565 1_545 ?
F4 Rb2 O2 72.3(3) 2_565 1_545 ?
O7 Rb2 O2 123.6(3) 3_545 1_545 ?
F5 Rb2 O2 87.6(2) 2_565 1_545 ?
O5 Rb2 O2 52.3(3) . 1_545 ?
F1 Rb2 O2 137.6(2) 4_565 1_545 ?
O10 Rb2 O2 90.6(3) 3_545 1_545 ?
O3 Rb2 O2 47.9(3) 1_545 1_545 ?
F6 Rb2 O8 80.2(3) 4_565 . ?
F4 Rb2 O8 123.9(3) 2_565 . ?
O7 Rb2 O8 56.4(3) 3_545 . ?
F5 Rb2 O8 71.2(3) 2_565 . ?
O5 Rb2 O8 47.1(3) . . ?
F1 Rb2 O8 119.4(3) 4_565 . ?
O10 Rb2 O8 94.1(3) 3_545 . ?
O3 Rb2 O8 123.6(3) 1_545 . ?
O2 Rb2 O8 99.3(3) 1_545 . ?
F6 Rb2 P1 152.0(2) 4_565 1_545 ?
F4 Rb2 P1 71.7(2) 2_565 1_545 ?
O7 Rb2 P1 122.9(2) 3_545 1_545 ?
F5 Rb2 P1 106.45(19) 2_565 1_545 ?
O5 Rb2 P1 76.7(2) . 1_545 ?
F1 Rb2 P1 111.40(19) 4_565 1_545 ?
O10 Rb2 P1 77.3(2) 3_545 1_545 ?
O3 Rb2 P1 26.28(19) 1_545 1_545 ?
O2 Rb2 P1 26.21(18) 1_545 1_545 ?
O8 Rb2 P1 122.2(2) . 1_545 ?
F6 Rb2 P2 100.3(2) 4_565 3_545 ?
F4 Rb2 P2 159.3(2) 2_565 3_545 ?
O7 Rb2 P2 24.7(2) 3_545 3_545 ?
F5 Rb2 P2 145.33(19) 2_565 3_545 ?
O5 Rb2 P2 96.1(2) . 3_545 ?
F1 Rb2 P2 66.81(17) 4_565 3_545 ?
O10 Rb2 P2 24.6(2) 3_545 3_545 ?
O3 Rb2 P2 76.6(2) 1_545 3_545 ?
O2 Rb2 P2 110.26(19) 1_545 3_545 ?
O8 Rb2 P2 76.6(2) . 3_545 ?
P1 Rb2 P2 101.31(9) 1_545 3_545 ?
F7 Rb3 O6 114.3(3) 2_565 1_545 ?
F7 Rb3 F5 58.5(3) 2_565 2_565 ?
O6 Rb3 F5 119.8(3) 1_545 2_565 ?
F7 Rb3 O9 132.3(4) 2_565 . ?
O6 Rb3 O9 94.3(3) 1_545 . ?
F5 Rb3 O9 74.3(3) 2_565 . ?
F7 Rb3 F1 55.8(3) 2_565 2_565 ?
O6 Rb3 F1 72.0(3) 1_545 2_565 ?
F5 Rb3 F1 110.3(2) 2_565 2_565 ?
O9 Rb3 F1 166.2(3) . 2_565 ?
F7 Rb3 O7 127.7(3) 2_565 1_545 ?
O6 Rb3 O7 49.6(3) 1_545 1_545 ?
F5 Rb3 O7 168.3(3) 2_565 1_545 ?
O9 Rb3 O7 100.0(3) . 1_545 ?
F1 Rb3 O7 72.9(3) 2_565 1_545 ?
F7 Rb3 O5 114.6(3) 2_565 . ?
O6 Rb3 O5 59.0(3) 1_545 . ?
F5 Rb3 O5 71.1(3) 2_565 . ?
O9 Rb3 O5 48.9(3) . . ?
F1 Rb3 O5 119.2(3) 2_565 . ?
O7 Rb3 O5 97.4(3) 1_545 . ?
F7 Rb3 O1 117.2(3) 2_565 3_445 ?
O6 Rb3 O1 102.8(3) 1_545 3_445 ?
F5 Rb3 O1 135.3(3) 2_565 3_445 ?
O9 Rb3 O1 90.2(3) . 3_445 ?
F1 Rb3 O1 94.6(2) 2_565 3_445 ?
O7 Rb3 O1 53.7(3) 1_545 3_445 ?
O5 Rb3 O1 127.8(3) . 3_445 ?
F7 Rb3 O3 119.1(3) 2_565 3_445 ?
O6 Rb3 O3 126.3(3) 1_545 3_445 ?
F5 Rb3 O3 93.0(3) 2_565 3_445 ?
O9 Rb3 O3 52.4(3) . 3_445 ?
F1 Rb3 O3 137.8(2) 2_565 3_445 ?
O7 Rb3 O3 91.4(3) 1_545 3_445 ?
O5 Rb3 O3 101.2(3) . 3_445 ?
O1 Rb3 O3 47.3(3) 3_445 3_445 ?
F7 Rb3 F4 164.7(3) 2_565 3_445 ?
O6 Rb3 F4 77.6(3) 1_545 3_445 ?
F5 Rb3 F4 125.4(3) 2_565 3_445 ?
O9 Rb3 F4 51.9(3) . 3_445 ?
F1 Rb3 F4 124.2(2) 2_565 3_445 ?
O7 Rb3 F4 51.9(3) 1_545 3_445 ?
O5 Rb3 F4 79.4(3) . 3_445 ?
O1 Rb3 F4 48.4(2) 3_445 3_445 ?
O3 Rb3 F4 48.8(2) 3_445 3_445 ?
F7 Rb3 P1 110.3(2) 2_565 3_445 ?
O6 Rb3 P1 125.4(2) 1_545 3_445 ?
F5 Rb3 P1 109.7(2) 2_565 3_445 ?
O9 Rb3 P1 77.2(2) . 3_445 ?
F1 Rb3 P1 111.97(18) 2_565 3_445 ?
O7 Rb3 P1 78.4(2) 1_545 3_445 ?
O5 Rb3 P1 124.7(2) . 3_445 ?
O1 Rb3 P1 25.81(19) 3_445 3_445 ?
O3 Rb3 P1 25.91(19) 3_445 3_445 ?
F4 Rb3 P1 54.55(16) 3_445 3_445 ?
F7 Rb3 P2 121.6(2) 2_565 1_545 ?
O6 Rb3 P2 24.9(2) 1_545 1_545 ?
F5 Rb3 P2 144.7(2) 2_565 1_545 ?
O9 Rb3 P2 100.7(3) . 1_545 ?
F1 Rb3 P2 67.80(18) 2_565 1_545 ?
O7 Rb3 P2 25.0(2) 1_545 1_545 ?
O5 Rb3 P2 79.4(2) . 1_545 ?
O1 Rb3 P2 78.7(2) 3_445 1_545 ?
O3 Rb3 P2 111.8(2) 3_445 1_545 ?
F4 Rb3 P2 65.14(18) 3_445 1_545 ?
P1 Rb3 P2 102.92(10) 3_445 1_545 ?
O4 Mn2 O3 178.1(5) 4_464 3_445 ?
O4 Mn2 F2 93.0(4) 4_464 . ?
O3 Mn2 F2 88.8(4) 3_445 . ?
O4 Mn2 O9 91.5(5) 4_464 . ?
O3 Mn2 O9 86.7(4) 3_445 . ?
F2 Mn2 O9 174.9(5) . . ?
O4 Mn2 O10 92.8(5) 4_464 . ?
O3 Mn2 O10 86.4(5) 3_445 . ?
F2 Mn2 O10 91.7(5) . . ?
O9 Mn2 O10 90.4(6) . . ?
O4 Mn2 F4 93.1(4) 4_464 3_445 ?
O3 Mn2 F4 87.7(4) 3_445 3_445 ?
F2 Mn2 F4 88.6(4) . 3_445 ?
O9 Mn2 F4 88.9(5) . 3_445 ?
O10 Mn2 F4 174.1(4) . 3_445 ?
O4 Mn2 Rb3 127.4(4) 4_464 . ?
O3 Mn2 Rb3 51.6(3) 3_445 . ?
F2 Mn2 Rb3 128.5(3) . . ?
O9 Mn2 Rb3 46.5(4) . . ?
O10 Mn2 Rb3 113.4(4) . . ?
F4 Mn2 Rb3 62.2(3) 3_445 . ?
O4 Mn2 Rb2 130.9(4) 4_464 3_455 ?
O3 Mn2 Rb2 49.3(3) 3_445 3_455 ?
F2 Mn2 Rb2 65.0(3) . 3_455 ?
O9 Mn2 Rb2 113.4(3) . 3_455 ?
O10 Mn2 Rb2 48.2(4) . 3_455 ?
F4 Mn2 Rb2 127.1(3) 3_445 3_455 ?
Rb3 Mn2 Rb2 98.48(6) . 3_455 ?
O4 Mn2 Rb1 105.7(3) 4_464 . ?
O3 Mn2 Rb1 72.4(3) 3_445 . ?
F2 Mn2 Rb1 132.6(3) . . ?
O9 Mn2 Rb1 47.8(4) . . ?
O10 Mn2 Rb1 45.3(4) . . ?
F4 Mn2 Rb1 131.9(3) 3_445 . ?
Rb3 Mn2 Rb1 71.44(5) . . ?
Rb2 Mn2 Rb1 70.00(5) 3_455 . ?
O4 Mn2 Rb2 57.4(4) 4_464 4_454 ?
O3 Mn2 Rb2 123.1(3) 3_445 4_454 ?
F2 Mn2 Rb2 99.7(3) . 4_454 ?
O9 Mn2 Rb2 80.8(4) . 4_454 ?
O10 Mn2 Rb2 148.3(4) . 4_454 ?
F4 Mn2 Rb2 37.2(3) 3_445 4_454 ?
Rb3 Mn2 Rb2 82.09(5) . 4_454 ?
Rb2 Mn2 Rb2 161.04(7) 3_455 4_454 ?
Rb1 Mn2 Rb2 127.18(6) . 4_454 ?
O4 Mn2 Rb1 59.4(3) 4_464 4_464 ?
O3 Mn2 Rb1 122.2(3) 3_445 4_464 ?
F2 Mn2 Rb1 35.4(3) . 4_464 ?
O9 Mn2 Rb1 149.6(3) . 4_464 ?
O10 Mn2 Rb1 83.3(4) . 4_464 ?
F4 Mn2 Rb1 100.3(3) 3_445 4_464 ?
Rb3 Mn2 Rb1 159.82(7) . 4_464 ?
Rb2 Mn2 Rb1 84.02(5) 3_455 4_464 ?
Rb1 Mn2 Rb1 127.47(5) . 4_464 ?
Rb2 Mn2 Rb1 89.15(5) 4_454 4_464 ?
F5 Mn3 O1 176.7(4) . . ?
F5 Mn3 F4 89.1(4) . . ?
O1 Mn3 F4 88.7(4) . . ?
F5 Mn3 O8 94.0(5) . . ?
O1 Mn3 O8 88.1(5) . . ?
F4 Mn3 O8 175.8(4) . . ?
F5 Mn3 O7 94.3(4) . 3_545 ?
O1 Mn3 O7 88.2(5) . 3_545 ?
F4 Mn3 O7 91.0(5) . 3_545 ?
O8 Mn3 O7 91.6(5) . 3_545 ?
F5 Mn3 F7 90.9(4) . . ?
O1 Mn3 F7 86.6(4) . . ?
F4 Mn3 F7 87.3(4) . . ?
O8 Mn3 F7 89.8(4) . . ?
O7 Mn3 F7 174.6(4) 3_545 . ?
F5 Mn3 Rb3 47.8(3) . 2_564 ?
O1 Mn3 Rb3 129.7(3) . 2_564 ?
F4 Mn3 Rb3 89.6(3) . 2_564 ?
O8 Mn3 Rb3 90.5(4) . 2_564 ?
O7 Mn3 Rb3 142.0(3) 3_545 2_564 ?
F7 Mn3 Rb3 43.2(3) . 2_564 ?
F5 Mn3 Rb1 129.9(3) . . ?
O1 Mn3 Rb1 50.6(3) . . ?
F4 Mn3 Rb1 129.2(3) . . ?
O8 Mn3 Rb1 46.7(3) . . ?
O7 Mn3 Rb1 113.1(3) 3_545 . ?
F7 Mn3 Rb1 64.5(3) . . ?
Rb3 Mn3 Rb1 95.44(7) 2_564 . ?
F5 Mn3 Rb3 129.2(3) . 3 ?
O1 Mn3 Rb3 51.5(3) . 3 ?
F4 Mn3 Rb3 63.0(3) . 3 ?
O8 Mn3 Rb3 116.6(4) . 3 ?
O7 Mn3 Rb3 48.8(4) 3_545 3 ?
F7 Mn3 Rb3 126.0(3) . 3 ?
Rb3 Mn3 Rb3 152.37(7) 2_564 3 ?
Rb1 Mn3 Rb3 99.35(6) . 3 ?
F5 Mn3 Rb2 46.7(3) . 2_564 ?
O1 Mn3 Rb2 132.0(3) . 2_564 ?
F4 Mn3 Rb2 46.4(3) . 2_564 ?
O8 Mn3 Rb2 137.5(3) . 2_564 ?
O7 Mn3 Rb2 78.5(3) 3_545 2_564 ?
F7 Mn3 Rb2 103.9(3) . 2_564 ?
Rb3 Mn3 Rb2 74.65(5) 2_564 2_564 ?
Rb1 Mn3 Rb2 168.38(7) . 2_564 ?
Rb3 Mn3 Rb2 87.50(6) 3 2_564 ?
F5 Mn3 Rb2 109.7(3) . . ?
O1 Mn3 Rb2 73.7(3) . . ?
F4 Mn3 Rb2 131.2(3) . . ?
O8 Mn3 Rb2 50.1(4) . . ?
O7 Mn3 Rb2 44.7(3) 3_545 . ?
F7 Mn3 Rb2 134.6(3) . . ?
Rb3 Mn3 Rb2 136.53(7) 2_564 . ?
Rb1 Mn3 Rb2 71.57(5) . . ?
Rb3 Mn3 Rb2 70.73(5) 3 . ?
Rb2 Mn3 Rb2 119.80(6) 2_564 . ?
 
_diffrn_measured_fraction_theta_max    0.997
_diffrn_reflns_theta_full              27.49
_diffrn_measured_fraction_theta_full   0.997
_refine_diff_density_max    1.370
_refine_diff_density_min   -1.222
_refine_diff_density_rms    0.293

